Copyright Warning & RestrictionsThe copyright law of the
United States (Title 17, United States Code) governs the making of
photocopies or other reproductions of copyrighted material. Under
certain conditions specified in the law, libraries and archives are
authorized to furnish a photocopy or other reproduction. One of
these specified conditions is that the photocopy or reproduction is
not to be used for any purpose other than private study,
scholarship, or research. If a, user makes a request for, or later
uses, a photocopy or reproduction for purposes in excess of fair
use that user may be liable for copyright infringement, This
institution reserves the right to refuse to accept a copying order
if, in its judgment, fulfillment of the order would involve
violation of copyright law. Please Note: The author retains the
copyright while the New Jersey Institute of Technology reserves the
right to distribute this thesis or dissertationPrinting note: If
you do not wish to print this page, then select Pages from: first
page # to: last page # on the print dialog screen
The Van Houten library has removed some of the personal
information and all signatures from the approval page and
biographical sketches of theses and dissertations in order to
protect the identity of NJIT graduates and faculty.
ABSTRACT SURFACE TREATMENT OF FERROUS ALLOYS WITH BORON by
Boronizing is a thermo-chemical surface hardening treatment in
which boron atoms diffused into the metal substrate form the
metallic boride layer, providing high hardness, corrosion
resistance, and 3-10 times increasing service life. This type of
surface treatment is widely used in many applications. The purpose
of this work was to investigate the structures and properties of
boronized ferrous alloys. Three types of steels, AISI 1018 (plain
low carbon steel), AISI 4340 (high strength alloy steel), and AISI
304 (austenitic stainless steel), were used for this study. The
boronized AISI 1018 and AISI 4340 demonstrated the saw-tooth
structure with average 75-76 pm and 57-58 AM in depth,
respectively. On the other hand, the narrow and flatten boride
layer with average 10-11 1.1.111 was observed in the boronized AISI
304. The microhardness of boride layer in AISI 1018 and AISI 4340
was detected in the range of 1400-2200 HV and 1800-2200 HV,
respectively, while that in AISI 304 was about 400-700 HV.
Moreover, unboronized steels showed the improved corrosion
resistance in acid and oxidation resistance at high temperature
rather than unboronized steels.
SURFACE TREATMENT OF FERROUS ALLOYS WITH BORON
by Naruemon Suwattananont
A Thesis Submitted to the Faculty of New Jersey Institute of
Technology in Partial Fulfillment of the Requirements for the
Degree of Master of Science in Materials Science and
Interdisciplinary Program in Materials Science and
APPROVAL PAGE SURFACE TREATMENT OF FERROUS ALLOYS WITH BORON
Dr. Roumiana S. Petrova, Dissertation Advisor Special Lecturer
of Physics, NJIT
Dr. Roland A. Levy, Committee Mem Distinguished Professor of
An Dr/ Federici, Committee Member Professor of Physics, NJIT
BIOGRAPHICAL SKETCH Author: Degree: Date: Naruemon Suwattananont
Master of Science August 2004
Undergraduate and Graduate Education: Master of Science in
Materials Science and Engineering, New Jersey Institute of
Technology, Newark, NJ, 2004 Master of Science in Materials Science
(Ceramic Technology), Chulalongkorn University, Bangkok, Thailand,
1996 Bachelor of Science in Chemistry, Chiang Mai University,
Chiang Mai, Thailand, 1993 Materials Science and Engineering
To my beloved family for their love, encouragement and support
especially, for their understanding in the way I am.
ACKNOWLEDGMENTI would like to express my deepest appreciation to
my advisor, Dr. Roumiana S. Petrova, who gave me the opportunity to
do this thesis and spent her time and offered for many suggestions
during the entire study. Special thanks are given to Dr. Roland A.
Levy and Dr. John Federici for actively participating in my
committee. Appreciation is also extended to all professors,
graduate students and staff of Physics Department, New Jersey
Institute of Technology. I would like to express my gratitude to my
family and boyfriend for their love, patience and encouragement and
also my appreciation for the research financial support from U.S.
Army ARDEC, Picatinny Arsenal, New Jersey.
TABLE OF CONTENTS Page
1 INTRODUCTION 1.1 Objective 1.2 Background Information 1.3 The
Trend of Surface Treatment with Boron 2 BORONIZING 2.1 Boromzing
(Boarding) 2.2 Boromzing of Ferrous Materials 2.3 Boromzing of
Nonferrous Materials 2.4 The Mechanism of Boromzing Process 2.5
Effects of Alloying Elements 2.6 Advantages and Disadvantages of
Boronizing 2.7 Application of Boromzed Products 3 BORONIZING
PROCEDURE 3.1 Pack Boromzing 3.2 Paste Boronizing 3.3 Liquid
Boronizing 3.4 Gas Boromzing 3.5 Plasma Boronizing 3.6 Fluidized
Bed Boronizing 3.7 Multi-component Boromzing
1 1 1 2 6 6 7 9 10 11 13 16 17 17 18 18 19 20 20 21
TABLE OF CONTENTS (Continued) Chapter 4 PROPERTIES OF BORONIZED
STEELS 4.1 Toughness 4.2 Adhesion Resistance 4.3 Adhesive Wear
Resistance 4.4 Corrosion Resistance in Acids 5 EXPERIMENTAL PARTS
5.1 Description of Experiments 5.2 Experimental Procedures 5.2.1
Sample Preparation 5.2.2 The Procedure of Boronizing Heat Treatment
5.2.3 Characterization of Boride Layers 5.2.4 Corrosion Testing
5.2.5 Oxidation Resistance Testing 6 RESULTS AND DISCUSSION 6.1
Characteristics of Boride Layer 6.1.1 Boride Layer 6.1.2 Phases
Present in the Boride Layer 6.1.3 The Morphology and Thickness of
Boride Layer 6.1.4 Microhardness 6.2 Corrosion Testing Page 23 23
23 23 25 26 26 27 27 27 29 31 32 33 33 33 34 37 39 40
TABLE OF CONTENTS (Continued) Chapter Page
6.3 Oxidation Resistance Testing 7 CONCLUSION 8 FUTURE WORK
APPENDIX A Fe-B PHASE DIAGRAM APPENDIX B Fe2B XRD DATA APPENDIX C
FeB XRD DATA REFERENCES
42 44 45 46 47 49 51
LIST OF TABLES Table2.1 The Microhardness and Constitution of
Bride Layers on Various Substrates Formed after Boronizing 2.2 The
Surface Hardness of Boromzed Steels Compares to Other Treatments
and Hard Materials 2.3 3.1 5.1 5.2 6.1 6.2 The Application of
Boronized Ferrous Materials The Multi-Component Boromzing The
Chemical Composition of Steel Samples The Grinding and Polishing
Procedure for the Steel Substrates The Boride Phase on the Specimen
Surface The Boride-layer Thickness on Steel Substrate 15 16 21 27
30 35 37 7
LIST OF FIGURES Figure 2.1 2.2 2.3 2.4 4.1 4.2 4.3 5.1 5.2 6.1
6.2 6.3 6.4 6.5 6.6 The saw-tooth structure of boride layers with
exterior layer FeB and interior layer Fe2B of AISI 1018 The effect
of steel composition on the morphology and thickness of the boride
layer The effect of percent alloying elements on the boride layer
thickness The hardness value for various materials and surface
treatments The effect of steel composition (nominal values in wt %)
on wear resistance under abrasive wear (4 = thickness of the boride
layer) The comparison of wear resistance between boromzed steels
and noneboromzed steel 24 The comparison of corrosion resistance
between boromzed steels and nonebronzed steels 25 The experimental
description flow chart The equipment setting for corrosion testing
(continuous weighting method) The image of AISI 1018 specimen
surface before and after boromzing The image of AISI 4340 specimen
surface before and after boromzing The image of AISI 304 specimen
surface before and after boromzing The XRD pattern of AISI 1018
before and after boronizing (P-unboronized Specimen, boromzed
specimen) The XRD pattern of AISI 4340 before and after boromzing
(P-unboromzed specimen, B-boronized specimen) The XRD pattern of
AISI 304 before and after boromzing (P-unboronized specimen,
B-boromzed specimen) 36 36 35 32 33 34 34 26 24 11 12 15 8 Page
LIST OF FIGURES (Continued) Figure 6.7 6.8 6.9 The saw-tooth
morphology and the distribution of the boride-layer thickness on
AISI 1018 The saw-tooth morphology and the distribution of the
boride-layer thickness on AISI 4340 The saw-tooth morphology and
the distribution of the boride-layer thickness on AISI 304 6.10 The
plot between the microhardness and the depth of boride layer in
AISI 1018 6.11 The plot between the microhardness and the depth of
boride layer in AISI 4340 6.12 The plot between the microhardness
and the depth of boride layer in AISI 304 6.13 The corrosion tests
of tmboronized and boromzed specimen (AISI 1018) in HC1 solution
(B- boromzed specimen, P-tmboromzed specimen) 6.14 The corrosion
tests of tmboronized and boromzed specimen (AISI 4340) in HC1
solution (B- boronized specimen, P-tmboromzed specimen) 6.15 The
corrosion tests of tmboromzed and boromzed specimen (AISI 304) in
HC1 solution (B- boromzed specimen, P-tmboronized specimen) 6.16
The oxidation test of boromzed and tmboromzed specimen (AISI 1018)
at 600 C for 12 hours (B- boronized specimen, tmboronized specimen)
6.17 The oxidation test of boronized and tmboronized specimen (AISI
4340) at 600 C for 12 hours (B- tmboronized specimen, P-unboronized
specimen) 6.18 The oxidation test of boromzed and tmboromzed
specimen (AISI 304) at 600 C for 12 hours (B- boromzed specimen,
P-tmboronized specimen) A.1 B-Fe (Boron-Iron) phase diagram 43 46
43 42 41 41 41 40 39 39 38 38 37 Page
CHAPTER 1 INTRODUCTION
The purpose of this work is to study the processing and
characteristics of boromzed steels. Three types of steel, AISI
1018, AISI 4340, and AISI 304, are investigated. AISI 1018, plain
low carbon steel, is widely utilized in many applications due to
the low cost; therefore, after boronizing the steel properties are
improved beneficial to the industry. Like AISI 1018, AISI 4340,
high strength alloy steel, is chosen to study due to the need of
better properties in aerospace industries. Finally, AISI 304,
austenitic stainless steel (18Cr8Ni), is used to compare the
results of boromzed AISI 1018 and boronized AISI 4340, according to
general uses in the industries and good properties in corrosion and
oxidation at high temperature.
1.2 Background Information
Boromzing is a well-known thermo-chemical surface hardening
treatment today. The boron atoms diffused into the metal substrate
can form the metallic boride layer on the metal surface, providing
high hardness, corrosion resistance, and 3-10 times increasing
service life 111 . Boronizing can complement the technology gap
between conventional heat treatment and chemical/physical vapor
deposition; therefore, it is used to replace many applications in
carburizing, nitriding, and carbonitriding 121 . However, only the
pack and paste boronizing techniques are able to process in many
other techniques, such as the liquid and gas boromzing
techniques, are incapable of the application because of toxicity
problems. Furthermore, the process can be applied to the irregular
surfaces or the specific areas of a surface. The high-volume
production applications are also available to process as first
demonstrated in the European automotive industry[31 .
As mentioned earlier,
boronizing fills out the gap between low and high technology;
hence the process provides low procedure cost but high quality
products, which is beneficial for the commercial section. In
addition, boromzing can combine with other heat treatments to
produce the multi-component boride layers that have the better
properties. The combination of excellent wear resistance, corrosion
resistance in acid, and oxidation resistance at high temperature is
one of the attractive features for the industrial application.
1.3 The Trend of Surface Treatment with Boron The trend of
surface treatment with boron can be classified into three
categories: 1. The advanced boronizing techniques In the last ten
years, the novel techniques were used to produce an efficient
boride layer on the substrate surface as discussed below: The laser
surface modification 141 was used to form the boride layer on 41Cr4
medium carbon steel. Although this method reduced the hardness of
the boride layer, it reduced the hardness gradient between the
boride layer and substrate. As a result, it caused the increasing
wear resistance in comparison with that of the conventional
3 The fluidized bed reactor was used to form the boride coating
0.5%wt. C steel,
nickel alloy [61 and nonferrous materials In. For this method,
the process could get the adequate thickness and improved wear and
oxidation resistances. Plasma Transferred Arc process (PTA)
technique, with using boron and chromium diboride powders, was used
to form iron-boron  and iron-chromium-boron [91 coatings. Both
coatings presented high hardness and excellent wear resistance.
Spark Plasma Sintering (SPS) technique1101
was able to avoid the drawbacks of
pack boromzing that took several hours during the boromzing and
of plasma-assisted boromzing that provided a high degree of
porosity on the boride layer. The plasma-assisted boromzing of
ferrous materials was formed under BC13H2 Ar atmosphere 1111 . The
treatment parameters and discharge conditions helped eliminating
the porosity of the boride layer. The plasma activation of
Ar-H2-BF3 atmosphere was also used to avoid the processing
corrosion " 21 . The D.C.-plasma boromzing technique combined with
PVCVD process achieved the deposition of boride layer at low
temperature (873 K)1131 .
The plasma paste boromzing  technique was processed on AISI
304. The boronizing paste had consisted of amorphous boron and
borax under gas mixture of Ar:H2 (2 : 1). The ion implantation
technique was processed on iron and AISI M2 steel along with using
a high current density, low-energy, and broad-beam ion source " 51
. The process provided thick boride layer while the boronizing
temperature was at 600 C for iron and at 700 C for steel.
4 2. The conventional boromzing technique In spite new boronized
techniques have been studied, many conventional techniques, such as
pack boromzing and salt bath, are still widely used to study on
many steels and their properties: in ductile iron 1161 , AISI W1
steel [171 , AISI 316L stainless steel[181 ,
AISI W4 steel 1191 , WC-Co steel [201 99.5% purity nickel,
alloy steels [221 , and etc. 3. Multi-component surface
treatment The multi-component of boronizing has widely been studied
to improve the mechanical properties, corrosion, and oxidation
resistances: Chromizing and boronizing treatment was combined to
increase the high oxidation resistance [231 . Boro-nitriding of
steel US 37-1 1241 was studied by combining two processes of pack
boromzing and gas nitriding to produce the boride, nitride and
boro-nitride layer with pore-free and excellent adherence. Vanadium
boride coatings on steel 1251 consisted of the thermo-diffusion of
vanadium and followed by boron. The microhardness of KB 2 was at
23600 MPa. B-C-nitriding in a two-temperature-stage process was
achieved to improve the boromzing embrittlement [261 . The complex
(B- C- N) diffusion layers (borocarbonitrided layer)  were
formed on chromium and nickel-based low-carbon steel. Despite the
Borocarbonitriding reduced the depth of iron boride zone, it
decreased microhardness gradient across the layer so that it
resulted in the low brittleness of the boride layer. The two-step
treatment carburizing followed by boronizing on medium-carbon steel
was fotmd to increase wear resistance and to decrease microhardness
The simultaneous boromzing and aluminizing produced tmder the
gas phase reaction of paste mixtures1291
was studied. The boroalutninized layers of C3, C5XHM,
X12, and X 1 8H9T steels [301 were investigated. The resulting
complex diffusion layers could be separated into three groups: the
needle-shaped layer with aluminium dissolved into iron boride, the
layer showing conglomerates of boride and aluminium phases, and the
layer with rich aluminium phases on the external surface. The
one-step boroaluminizing heat treatment was studied on 2.25CrMo
steel [311 by means of pack cementation technique using a B/A1
boronizing powder. Three distinct regions were fotmd in the
coatings: first, an outer Al-rich layer region, second, a
transition region containing A1 and Fe, and third, an inner layer
region containing mostly B and Fe. The boroaluminizing improved the
oxidation and hot corrosion resistance. The multi-component of
Ni4B3, (Fe,Ni)B, and (Fe,Ni)2B borides
by combining the electrochemical nickel deposition and plasma
boronizing to increase the wear and corrosion resistance of
CHAPTER 2 BORONIZING
2.1 Boronizing (Boarding)
Boronizing is a thermo-chemical surface hardening process that
boron atoms diffuse into a base metal (steel) and form the hard
metallic boride layer on the surface. The process can be applied to
both ferrous and nonferrous materials by heating well-cleaned
materials in the temperature range of 700 - 1000C (1300 - 1830F)
for several hours. The process provides the metallic boride layer
about 20-300 gm thick. The resulting metallic boride layer yields
the outstanding properties of high hardness, good wear and
corrosion resistance, and moderate oxidation resistance at high
temperature. Although many metals and alloys can be boromzed,
aluminium and magnesium alloys cannot be boromzed due to their low
melting points. In addition, copper alloy is unable to form the
stable boride phase  . During boronizing, boron atoms diffuse
and subsequently absorb into the metallic lattice of the component
surface. As a result, an interstitial boron compotmd is formed with
either a single-phase boride or a poly-phase boride layer. Several
characteristics of the boride layer, including the morphology, the
growth, and the phase composition, depend on the elements in the
substrate materials (Table 2.1).
7 Table 2.1 The Microhardness and Constitution of Boride Layers
on Various SubstratesFormed after Boronizing [331
2.2 Boronizing of Ferrous MaterialsThe boride layer formed on
iron and steel can be of either a single phase or double-phase,
corresponding to a definite composition from Fe-B phase diagram
(Appendix A). Fe2B is obtained for the single-phase layer, while
the double-phase layer consists of an exterior phase of FeB and
interior phase of Fe2B, whereas the morphology of the boride layer
saw-tooth structure as shown in Figure 2.1. The saw-tooth
structure helps improving the mechanical adherence at the Fe 2
Figure 2.1 The saw-tooth structure of boride layers with
exterior layer FeB and interior layer Fe2B of AISI 1018.
Because FeB phase is more brittle than Fe2B phase, the formation
of Fe2B phase is expectedly preferred than that of FeB phase. In
addition, it is observed that Fe2B forms a surface under the high
compressive stress, while FeB forms a surface under the high
tensile stress. However, the boronizing process avoids having the
coincidence of Fe 2 B and FeB phases, which causes to the crack
formation at the FeB/Fe2B interface of doublephase layer. The crack
formation leads to the spalling and even the separation of
doublephase layer under the applied mechanical strain or the
thermal/mechanical shock. Fortunately, the annealing process can
decrease the occurrence of FeB phase after boronizing treatment
rile. The characteristics of the Fe 2 B phase include Composition
with 8.83 wt% boron Body-centered tetragonal crystal structure
(a5.078A, c4.249A) Density of 7.43 g/cm 3 Microhardness of about
18-20 GPa[341 :
9 Yotmg's modulus of 285-295 GPa Thermal expansion coefficient
of 7.65x10 1C in the range 200-600 C, and 9.2x10 -6 /C in the range
100-800 C The characteristics of the FeB phase include  :
Composition with 16.23 wt% boron Orthorhombic crystal structure
(a=4.053A, b=5.495A, c=2.946A) Density of 6.75 g/cm 3 Microhardness
of about 19-21 GPa Young's modulus of 590 GPa Thermal expansion
coefficient of 23x10 -6 /C in the range 200-600 C
2.3 Boronizing of Nonferrous MaterialsRefractory metals,
titanium, nickel, cobalt and their alloys can be boromzed by using
special techniques such as gas and plasma boromzing, instead of
conventional boronizing techniques. Since the salt bath and
conventional powder boromzing techniques are inapplicable for
titanium and refractory metals because of the oxidation on the
substrate and the corrosion from the activator that cause the
porosity in the boride layer1331 .
Therefore, the heat treatment for refractory and titanium metals
is required to be operated tmder high vacuum and high purity argon
atmosphere, or with the gas (H2 - BC 1 3) boronizing technique. For
the refractory metal and titanium, the process is prepared at the
temperature above 1000 C for 10-15 hr[331.
The resulting boride layer is about 50 pm thick with
high microhardness values (Table 2.1). However, the boride layer
of tantalum, ttmgsten,
niobium, molybdenum, and nickel metal does not show the strong
saw-tooth structure as seen in titanium and cobalt metal1341 .
Furthermore, the saw-tooth structure in nonferrous
materials is not manifestly when compared to that in ferrous
materials (low/medium carbon alloy).
2.4 The Mechanism of Boronizing Process
The boronizing process consists of two reactions: 1. The initial
stage takes place between boron medium and component surface. The
nuclei are formed as the ftmction of boronizing temperature and
time and are followed by the growth of boride layer  . In case
of ferrous materials135361 ,
nuclei are first formed and grow a thin boride layer at the
defect points of the metal surface, macrodefects (surface
roughness, scratches, etc.) and microdefects (grain botmdaries,
dislocation, etc.). If the active boron medium is excess, the rich
boron product phase, such as Fe8, will form and grow on the Fe28
phase. 2. The second stage is a diffusion-controlled process, which
the thickness of bride layer is formed tmder a parabolic time
x2 = kt
where x as the thickness of the bride layer, k as a constant
depending on the temperature, and t as the boronizing time 1341 .
In case of ferrous materials, boron atoms prefer to diffuse in the
 crystallographic direction and form the body-centered
tetragonal lattice of Fe28 to achieve the maximum atomic density
along this direction135-
The growth of Fe2B is columnar aggregates of crystals, which
exhibits the saw-tooth
morphology. For the double phase, the columnar growth of FeB
prefers to grow in the  crystallographic direction and the
saw-tooth structure of FeB is lower than that of Fe2B.
2.5 Effects of Alloying Elements
The prominent saw-tooth structure of boride layer is well
observed in pure iron, unalloyed low-carbon steel, and low alloy
steels. When the alloying elements and/or carbon contents in the
substrate steel are increased, the thickness of the boride layer is
reduced. In addition, the smooth interface may be observed instead
of the saw-tooth structure illustrated in Figures 2.2 and 2.3.
Another effect of alloying elements (except nickel, cobalt, and
manganese), which retard the boron diffusion into the substrate, is
to increase the proportion of FeB constitutionI33] .
For example in boronized stainless steel,
the consequence of alloying elements leads to the thin smooth
interface with almost 100% FeB formation of boride layer.
Figure 2.2 The effect of steel composition on the morphology and
thickness of the boride layer.
Figure 2.3 The effect of percent alloying elements on the boride
layer thickness 121 .
Carbon, Silicon, and Aluminum is insoluble in the boride layer.
During the boronizing, the boride layer will drive carbon and
silicon away from the surface to the substrate matrix and forms the
precipitation of iron silicoboride (FeSi 0.480.6 or FeSi82) and
iron carboboride (Fe23(8,C)6 and Fe3(8,C) beneath and/or between
the boride sawteeth structure. The contents of silicon and
aluminium (larger than 0.8%) tmderneath the boride layer can form a
soft ferrite phase, which has a low load-carrying capacity 1371 .
Under the high surface pressure, the failure can occur due to the
hard boride layer penetrating into this soft ferrite region. Nickel
will restrict the solubility of boron atoms in iron by diffusing
into the boride layer and by precipitating Ni38 from the boride
layer at the Fe28/substrate interface. The result is the reduction
of boride-layer thickness and saw-tooth structure. Although nickel
may slightly reduce the microhardness value of the boride layer,
nickel helps impeding the formation of Fe8 1371 .
13 Chromium is a modifier for the structure and properties of
boride layer. The
solubility of chromium in the Fe28 phase causes the replacement
from iron to chromium and forms (Fe,Cr)8 and (Fe,Cr)28 on the
surface. The incorporation of chromium may increase the
microhardness of boride layer but it causes boron to diffuse along
the grain boundaries. The diffusion leads to the decreasing of
boride layer thickness and the increasing of the smooth boride
r371 . Chromium also promotes
the formation of rich boron product phase, such as Fe8, to the
boride layer.Manganese, Tungsten, Molybdenum, and vanadium are
typically to reduce the
boride thickness and flatten out the saw tooth morphology.-
2.6 Advantages and Disadvantages of Boronizing Advantages:
The boronized steels can provide the extremely high hardness,
compared with other treatments and other hard materials as listed
in Table 2.2 and Figure 2.4.
The combination of a high surface hardness and a low surface
coefficient of friction in boromzed steel provides the outstanding
of wear mechanisms, including adhesion, tribooxidation, abrasion,
and surface fatigue.
The surface hardness of boromzed steel can retain at high
temperature. The process can be applied to a variety of metals and
alloys. 8oromzed surfaces of ferrous materials have a high
corrosion-erosion resistance in dilute acid and alkali media and
are available in the industrial applications.
8oromzed surfaces have a moderate oxidation resistance (up to
850 C or 1550 F).
14 8oromzed surfaces are resistant to the attacks by molten
metals. The boromzed steels can increase the fatigue life and the
service performance tmder the normal application and oxidation or
Disadvantages: The technique is inflexible and rather
labor-intensive. Therefore, the process is less cost-effective than
other thermo-chemical treatments. The boride thickness cannot be
well controlled because the thickness growth depends on the
substrate composition and the consistency of boromzed powder
composition. The formation of boride layer increases the dimension
of the base metal. The removal of the boride layer in order to meet
the closer tolerance requirements is required to use the diamond
lapping, since the conventional grinding causes the fracture of the
15 Table 2.2 The Surface Hardness of 8oromzed Steels Compares to
Other Treatments and Hard Materials [21
16 2.7 Application of Boronized Products
The conclusive boromzed parts have been widely used in a variety
of industrial applications as shown in Table 2.3.
CHAPTER 3 BORONIZING PROCEDURE
3.1 Pack Boronizing The pack boromzing or solid state boronizing
technique is the most widely favored technique due to the
simplicity and economy. The process involves the embedding of the
metals/alloys into the boronizing powder mixture that consists of
three substance groups:
Boron source: Boron carbide (134C), ferroboron, and amorphous
boron Activator: Na8F4, KBF 4 , (NH4)3BF4, NH 4CI, Na2CO3, BaF2,
and Na2B407 Diluent: SiC, Al203
In the heat-resistant container, the well-cleaned and smooth
metals/alloys are packed in the boromzing powder mixture with 10-20
mm thick and 50-100 mm deep, and covered by a container lid. The
heat treatment is processed in the furnace. After reaching the
boronizing temperature and time, the container is then removed from
the furnace and allowed to cool down at room temperature. To avoid
the adverse effect of oxygen on boromzing, the boronizing treatment
should be performed tmder the protective-gas atmosphere, such as
or mixture of Ar-N2-H2. The protective-
gas must be maintained after boronizing until the process is
cooled down to 300 C (570 F) Using the above procedure, the
boronizing powder mixture can be reused about 56 times by blending
in 20-50% with the new powder mixture.
18 3.2 Paste Boronizing The paste boromzing technique is
practical for the large components or partially or selectively
required part of components. The boromzing paste consists of 55%84C
(grain size 200-240pm) and 45%cryolite (Na3AIF6)1301 ,
or the traditional boromzing powder
mixture (84C-SiC-KBF4) with the binder, such as nitrocellulose/
butyl acetate, methylcellulose, or hydrolyzed ethyl silicate1331
The method to apply the paste can be
dipping, brushing, or spraying with the thick layer about 1-2 mm
and is processed under the protective-gas atmosphere. After the
heat treatment, the boromzing paste is removed by blast cleaning,
brushing or washing.
3.3 Liquid Boronizing The liquid boromzing or salt bath
boromzing technique is performed in the borax-based salt melts
(Na28 4 O7) with and without electrolysis at the temperature above
900 C1331 .
The technique is suitable for the complex body. The component
must resist to the thermal shock of immersion and removal from the
bath to prevent the component deformation and cracking. After
treatment, the excess melting salt must be removed from the
component, causes the high cost and time consuming. The maintenance
cost is also high because the process requires the salt recharging
for the appropriate viscosity to prolong the boromzing reaction.
The corrosive fume from the reaction creates another problem to the
technique. Electroless liquid boronizing: The common salt bath is
30-70% Borax-84C and the reaction is enhanced by replacing 20% 84C
with ferroaluminium because of the
effective reductant. For the nickel alloy, the bath is composed
of 75%wt KBF4 - 25%wt KF, operating at temperature below 670 C.
Electrolytic liquid boronizing: The component is attached to a
while the graphite is acted as an anode. Both of them are
immersed in the molten borax at 940 C and the current (0.15A/cm 2 )
is passed to them. At the liquid state, Borax is decomposed to
sodium ions (Nat) and tetraborate (13407 2 ). The reaction is as
3.4 Gas Boronizing
The gas boromzing technique is a diffusion process of some gas
media, such as diborane (82H6) or boron chloride (BC13). This
method is tmavailable for the industry concerned by the toxic and
the explosion of gas media. The BC13-H2 gas mixture has previously
been attempted to boronize the steel, but the high concentration of
BCl3 causes the corrosion on the substrate and results the poor
adherent layers. To improve the technique, the dilute (1:15)
BC13-H2 gas mixture is commonly used at 700- 900 C and under the
pressure of about 67 kPa 1391 . Moreover, the replacing of a
carrier-reductant gas of 75%N2 and 25%H2, rather H2, can reduce the
BC13 concentration. As a result, it avoids FeCl3 (corrosion) and
diminishes the Fe8 formation. As well, this process can be used
with titanium and its alloys.
20 3.5 Plasma Boronizing The plasma boromzing technique is not
yet available in the commercial application because of the same
problems as occurred in the gas boromzing technique. The gas
mixtures of 82H6H2 and BCl3-H2-Ar are used in this technique.
Additionally, theBC13H2-Ar gas mixture exhibits good features of
controlling an amotmt of BC13 concentration. The resulting features
reduce the discharge voltage and increase the microhardness of the
boride layer 1401 . Despite the porosity of double-phase boride
layer is observed, increasing the BC13 concentration can minimize
it. This technique is widely applied to the refractory metals
because of the high-efficient deposition of the boride layer, which
is higher than that of the pack boronizing technique. By this
technique, the process can be operated at the low temperature 600 C
(1100 F) and in the short time, which helps saving in energy and
gas consumption. The conventional pack boromzing technique,
however, cannot operate at such low temperature.
3.6 Fluidized Bed Boronizing The fluidized bed boromzing
technique is a recent innovation of boromzing. The bed materials,
coarse-grained silicon carbide and boromzing powder mixture, are
served as a faster heat-transfer medium through which an
oxygen-free gas (N2-H2) flows. The high heating rate and high
flowing rate provide the rapid boronizing, meaning the shorter
operation time. Because of the temperature tmiformity, the process
can also produce the reproducibility, good tolerances, and tmiform
finishing mass-products. Finally, this technique achieves the low
operating cost for the mass production of boromzed parts. However,
the major disadvantage is the exhaust gases (fluorine compotmds)
that must be
completely eliminated by using the CaCO3 absorber to avoid the
3.7 Multi - component Boronizing The multi-component boromzing
technique is the process that combines the diffusion of boron and
one or more metallic element(s), including aluminium, chromium,
vanadium, and silicon, into the substrate surface. Some
multi-component boronizing systems are illustrated in Table 3.1.
The multi-component boromzing can be classified into three types
Type 1: simultaneous boromzing and metallizing Type 2: boromzing
followed by metallizing Type 3: metallizing followed by
22 The attracting result from this process is an improvement of
mechanical properties and oxidation resistance as stated below:
Boroaluminizing the compact layer provides good wear and
resistance, especially in humid environments Borosiliconizing
the FeSi is formed on the boride-layer surface that
increases the corrosion-fatigue strength of component.
Borochromizing this treatment provides the better oxidation
boroaluminizing, gives the uniform layer, improves the wear
resistance, and increases the corrosion-fatigue strength.
Borovanadized and borochromvanadized the layer will have ductility
high microhardness (>3000HV at 15g load), which helps
reducing the spalling tmder the impact loading condition.
CHAPTER 4 PROPERTIES OF BORONIZED STEELS
After boronizing, steels will have the desirable properties on
the surface, including the increasing wear resistance, corrosion
resistance, and 3-10 times increasing service life.
4.1 Toughness The boride layer provides the good bonding with
the base metal, which can ensure that tmder load, the flaking or
the peeling will not happen. However, the toughness of the boromzed
steel relies on its boride layer thickness, cross-section area, and
mechanical properties. In the bending test, the boronized sample
with the boride-layer thickness of 150-200 p.m has 4% elongation
without cracking i l l.
4.2 Adhesion Resistance The boromzed surfaces show neither
accretion nor wear of material as well as having hardly any
tendency to cold-weld 1371 . Consequently, this property is used in
the coldmetal working (chipless shaping) as a tool to form the
metals. Without the non-lubricant, the boronized layers do not have
an appreciable change at 300 C in order to protect the environment
by reducing the lubricant.
4.3 Abrasive Wear Resistance High microhardness provides high
wear resistance. Some resulting properties of boronized steels are
shown in Figures 4.1 and 4.2.
Figure 4.2 The comparison of wear resistance between boronized
steels and nonboronized steel 121 .
25 4.4 Corrosion Resistance in Acids
Boromzed carbon and alloy steel have the increasing corrosion
resistance in HCI, H2SO4, and H3PO4. The boronized austenitic
stainless steel improves the corrosion resistance in CI as shown in
CHAPTER 5 EXPERIMENTAL PARTS
5.1 Description of Experiments The steel samples (AISI 1018,
AISI 4340, and AISI 304) were chosen to boronize at 850 C for four
hours tmder the argon atmosphere. The boride layer of boromzed
steel samples was characterized in terms of phase identification,
thickness, morphology, and microhardness. The corrosion resistances
of both tmboronized and boronized steel samples were observed as
well as the oxidation resistance. The experimental flow chart was
illustrated in Figure 5.1.
27 5.2 Experimental Procedures The experimental procedures were
described as below:
5.2.1 Sample Preparation AISI 1018, AISI 4340, and AISI 304
samples were cut in the dimension of 10 x 10 x 3 mm, 12 x 12 x 7
mm, and 12 x 10 x 6 mm, respectively. The chemical composition of
sample steels was shown in Table 5.1. Firstly, the samples were
grinded with the 120, 220, 400, and 600-grit sand papers. The
samples, then, were cleaned with acetone in the ultrasonic bath for
5-10 minutes and dried in the air.
5.2.2 The Procedure of Boronizing Heat Treatment The boromzing
heat treatment procedures can be classified into three steps.
18.104.22.168 The Preparation of Boronizing Powder Mixture. The
mixture was prepared by mixing together 1% w/w KBF4 (potassium
tetrafluoroborate, 99% min (assay), typically >99.5% (assay) of
Alfa Aesar), 5% w/w Al203 (aluminum oxide powder, 99.99%, 20-30
micron of Atlantic Equipment Engineers), and 94% w/w 84C (boron
carbide, 240 grit, technical grade of Electro Abrasives
Corporation). KBF4 and Al203 were first mixed in the mortar to
break the powder cluster and followed by
28 gradually adding a small quantity of 84C to prevent the
segregation of KBF4 and Al203 powder from 84C into the gradients.
After all substances were mixed in the mortar, the boronizing
powder mixture was mixed again in the blender to be confident that
the component was well homogeneous. 22.214.171.124 The Packing of
Boronizing Powder. The boromzing power mixture was dried at 250 C
for two hours in the box furnace (ThermoLyne model 48015). The
wellcleaned sample steels were embedded in the boronizing power
mixture contained in inconel crucible. After the boromzing powder
mixture was filled full in the crucible, the crucible should be
tapped until the powder mixture was densely packed. It was to
prevent the air trap among the powders. Sequentially, the crucible
full-filled with powder mixture was degassed overnight
(approximately 12 hours) in the desiccator that connected to the
vacuum system. 126.96.36.199 The Boronizing Heat Treatment. The crucible
containing the boromzing powder mixture and the embedded sample
steels was dried for two hours at 250 C in the furnace. After that,
the crucible lid was covered tightly. Then, the furnace temperature
was increased to 850 C and was held for four hours in the argon
atmosphere (Argon (99.999%) of SOS Gases) with the flow rate 60
psi. After reaching the required temperature and time, the furnace
was cool down to 300 C tmder the argon atmosphere and the furnace
was switched off. When the furnace was cool down to the room
temperature, the boromzed sample steels were removed from the
crucible and were cleaned with the methanol in the ultrasonic
29 5.2.3 Characterization of Boride LayersThe boride layers were
analyzed with three aspects as follows.
188.8.131.52 Phase Identification. The X-ray Diffraction Method (XRD)
was used toinvestigate the tmboromzed and boromzed sample steel
phases of AISI 1018, AISI 4340, and AISI 304. XRD Philips (PW3040
MPD DY715) was used tmder the system condition as followed: the XRD
wavelength utilized was Cu K-a 1 (1.5405980 A) at 45 kV and 40 mA;
the '/2" divergence slit, '/2" anti-scatter slit, and 15 cm mask
were chosen to detect the XRD spectrum; the 20 scan range was from
20-100 with step size of 0.020 and 2.70 times per step. The
specimen phase was analyzed by using X'Pert high score
184.108.40.206 Morphology and Thickness. The outer surface of boromzed
sample steelswas observed by using optical microscopy. The AxioTech
Microscope of Carl Zeiss with 10x eyepiece lens and 20x, 50x, 100x
objective lens was used to investigate with Differential
Interference Contrast (DIC), Darkfield, and Brightfield methods.
The resulting microstructure images have been taken by using the
digital camera (Pixelink PL-A662). The cross-sectional specimen was
used to examine the thickness and morphology of the boride layers
penetrating into the steel substrates. The boronized sample steels
were motmted with the epoxy resin (EpoxyMotmt of Allied High Tech
Products, Inc.) in the two-part motmting cups. The mixing ratio of
part A (resin) and part B (hardener) was 100:30 by weight. After
motmted, the specimens were placed in the desiccator and degassed
tmder the vacuum system for 10 minutes. They were then left to cure
30at room temperature and thereafter were removed from the
mounting cups and continued with the grinding and polishing
procedures. The grinding and polishing machine (MetPrep3 from
Allied High Tech Products, Inc.) was deployed. The grinding and
polishing procedures are demonstrated in the Table 5.2.
After grinded and polished, the specimens were cleaned with
water in the ultrasonic bath until all substances remaining from
the polishing procedure was completely eliminated. They were dried
with the air blower. To observe the morphology and thickness of
boride layers, the AISI 1018 and AISI 4340 specimens would be
etched by the etching solution of 0.5g picric acid (98% picric acid
of Aldrich), 12.5g sodium
31 hydroxide (>98%(assay) sodium hydroxide of Fluka), and
25m1 distilled water at 35 40 C for one minute, while AISI 304
specimens were etched in 3% nitric acid. After etching the
specimens were washed with water in the ultrasonic bath. It should
not have any etching solution left on the specimen surface because
the etching solution caused the distortion of the image color.
After that, the morphology microstructure of boride layers was
observed with the optical microscope and the microstructure images
were taken. The thickness of the boride layer was measured by using
AxioVision Software Version 4.1 of Carl Zeiss. The measurement of
each saw-tooth structure depth was randomly examined. Subsequently,
the distribution and average value of thickness depth were
calculated by using the statistic operation. 220.127.116.11 Microhardness.
The microhardness of boronized sample steels (AISI 1018, AISI 4340,
and AISI 304) was determined at every boride-layer depth by using
LM700 Microhardness Tester with the Vickers indenter of Leco. The
relationship between the Vickers microhardness and the boride layer
depth was observed. 5.2.4 Corrosion Testing The corrosion
resistances of tmboronized and boromzed sample steels (AISI 1018,
AISI 4340, and AISI 304) were investigated by a continuous
weighting method. The weight loss of the specimen was continuously
detected as a ftmction of time. The 5%, 10%, 15% w/w hydrochloric
acid (HC1) were used as corrosive media. The setting equipment for
this experiment was illustrated in Figure 5.2.
From Figure 5.2, the specimen was htmg down from the balance
(Analytical Balance GR-202 of A&D) with platinum wire and
immersed in hydrochloric acid solution for 24 hours. The specimen
weight was detected every 36 seconds and automatically stored in
5.2.5 Oxidation Resistance TestingThe oxidation resistance of
tmboromzed and boromzed steels (AISI 1018, AISI 4340, and AISI 304)
was investigated at 600 C for 2, 4, 6, 8, 10, 12 hours in the box
furnace. The weighted specimen was placed inside the ceramic boat
and then put into the furnace. Periodically every two hours, the
specimen was removed from the furnace, cooled down at room
temperature, and weighted. The weight gains of specimen were
detected with respect to the soaking time.
CHAPTER 6 RESULTS AND DISCUSSION
6.1 Characteristics of Boride LayerThe analysis of boride layer
shows the major characteristics into four aspects.
6.1.1 Boride SurfaceAfter the boronizing heat treatment, the
sample surface was seen in dark grey color, which was a color of
iron-boron compound (FeB and Fe 2 B). The image of specimen's
surface before and after boronizing heat treatment was illustrated
in Figures 6.1, 6.2 and 6.3. From these figures, it was indicated
that the boride layer that occurred during the boronizing process
increased the roughness of specimen's surface. Consequently, the
roughness might be the problem of low specimen tolerance.
a) The specimen surface before boronizing
b) The specimen surface after boronizing
Figure 6.3 The image of AISI 304 specimen surface before and
6.1.2 Phases Present in the Boride Layer
To detect the occurrence of boride-layer phases on the boromzed
specimen, the XRD pattern of unboronized specimen was used as a
background phase. The different boridelayer phases deposited on the
specimen surface after boronizing were shown in Table 6.1.
35The XRD patterns of AISI 1018, AISI 4340, and AISI 304 were
shown in Figures 6.4, 6.5, and 6.6, respectively.
Figure 6.4 The XRD pattern of AISI 1018 before and after
boronizing (P-unboronized specimen, B-boronized specimen).
Figure 6.6 The XRD pattern of AISI 304 before and after
boronizing (P-unboronized specimen, B-boronized specimen).
376.1.3 The Morphology and Thickness of Boride Layer
The saw-tooth structure or the needle-like structure of boride
layer penetrating into the substrate matrix was observed on the
cross-sectional specimen. The microstructure image of inward Fe2B
phase and outward FeB phase was exhibited in brown color and blue
color, respectively. The average boride-layer thickness of AISJ
1018, ATSI 4340, and AISI 304 was shown in Table 6.2. The
distribution of the boride-layer thickness and the cross-sectional
specimen morphology were also shown in Figures 6.7, 6.8, and
Figure 6.7 The saw-tooth morphology and the distribution of the
boride-layer thickness on AISI 1018.
Figure 6.9 The saw-tooth morphology and the distribution of the
boride-layer thickness on AISI 304.
According to the chemical composition of steels in Table 5.1, it
was seen that the boride-layer thickness was inverse to the
alloying elements in the sample steels. The increasing of alloying
elements caused the decreasing of boride-layer thickness. AISI
1018, plain carbon steel without alloying elements, demonstrated
the saw-tooth structure with 75 76 [tam in depth, while AISI 4340,
high strength alloy steel, had more alloying elements than AISI
1018, showing the shorter saw-tooth structure of boride layer (57 -
58 Inn). In case of AISI 304 (austenitic stainless steel), the
narrow (10 -11 Jim) and smooth boride layer was detected, which was
the effect on the high quantities of chromium and nickel as
alloying elements in AISI 304 steel substrate.
39 6.1.4 Microhardness
The microhardness of boride layer related to the amount of boron
atoms that diffused into the substrate, in terms of the depth from
the external surface. The fact that microhardness decreased as the
depth from the surface increased was observed and illustrated in
Figures 6.10, 6.11, and 6.12. Moreover, it was shown that the
decline of microhardness became larger on going towards to the bulk
of the substrate.
Figure 6.11 The plot between the microhardness and the depth of
boride layer in AISJ 4340.
Figure 6.12 The plot between the microhardness and the depth of
boride layer in AISI 304.
6.2 Corrosion Testing
The corrosion resistance testing of boronized specimen was
investigated in 5%, 10%, and 15% w/w hydrochloric acid, compared
with that of unboronized specimen in 5% w/w hydrochloric acid. The
unique technique (continuous weighting method) was used to
investigate the results of corrosion resistance. For AISI 1018, the
boronized sample was able to resist in 5% w/w hydrochloric acid but
it could not protect the substrate from the acid corrosion in 10%
and 15% w/w hydrochloric acid as shown in Figure 6.13. For AISI
4340, the boronized steel also enabled to protect the substrate
from the corrosive media as shown in Figure 6.14. Especially, AISI
304, which usually could not persist in hydrochloric acid, was able
to resist in hydrochloric acid as shown in Figure 6.14.
Figure 6.15 The corrosion tests of unboronized and boronized
specimen (AIST 304) in HC1 solution (B-boronized specimen,
42 6.3 Oxidation Resistance Testing
The oxidation resistance of boronized and unboronized specimens
was determined at 600 C for 12 hours. In case of AISI 1018
illustrated in Figure 6.16, the experimental result showed that the
oxidation resistance of boronized specimen was higher than that of
unboronized specimen about three times. In case of AISI 4340
illustrated in Figure 6.17, during the beginning of experiment the
oxidation resistance of boronized specimen was higher than that of
unboronized specimen; however, after 8 hours the oxidation
resistance of boronized specimen seemed constant while the
unboronized specimen inclined continuously. In case of AISI 304
illustrated in Figure 6.18, the results showed the better oxidation
resistance of boronized specimen than that of unboronized
Figure 6.16 The oxidation test of boronized and unboronized
specimen (AISI 1018) at 600 C for 12 hours (B-boronized specimen,
Figure 6.17 The oxidation test of boronized and unboronized
specimen (AISI 4340) at 600 C for 12 hours (B-boronized specimen,
Figure 6.18 The oxidation test of boronized and unboronized
specimen (AISI 304) at 600 C for 12 hours (B-boronized specimen,
CHAPTER 7 CONCLUSION
The boronized specimens of AISI 1018, AISI 4340, and AISI 304
were successfully prepared by the pack boromzing technique. The
investigation of structure and properties of boride layer in
ferrous alloys was concluded as followed: 1. AISI 1018, plain low
carbon steel, showed the saw-tooth structure with the depth of
about 75 76 1.1111. The boride layer was consisted of an outer FeB
phase layer and an inner Fe28 phase layer. The microhardness was
obtained in the range of 14002200 HV. 2. Similar to AISI 1018, AISI
4340, high strength alloy steel, also demonstrated the saw-tooth
structure with the depth of about 57 - 58 gm. Fe8 and Fe28 phase
were detected as a boride layer on the substrate. The microhardness
was recorded in the range of 1800-2200 HV. 3. Unlike AISI 1018 and
AISI 4340, the narrow and flatten boride layer (10 11 gm) was
observed instead of the saw-tooth structure, as a result of
alloying elements, particularly chromium and nickel in AISI 304.
The microhardness of boride layer in AISI 304 was about 400-700 HV.
4. The new tmique technique was used to evaluate the corrosion
resistance and boromzed sample steels showed the ability of the
boromzed coating to protect the substrate. 5. The boromzed
specimens also showed the improved of oxidation resistance at high
temperature rather than the tmboromzed specimens.
CHAPTER 8 FUTURE WORKSince the pack boronizing is the simplest
boronizing technique to tmderstand the basic principle required for
advance research on developing boromzed steel, other boronizing
techniques are planned to study and yet realize the optimized
properties. 1. The gas and plasma boronizing utilizes the gas
medium, rather than the solid powder in the pack boromzing method,
with appropriate and controllable procedures to produce the
optimized properties. 2. The multi-component boromzing is expected
to construct the complex phase boride-layer that in general yields
the desired properties. 3. The boromzing process for transition
metals and their corresponding properties, which are deployed in
extremely hard-surface applications, will be investigated.
APPENDIX B Fe2B XRD DATA
The crystallography data and XRD pattern of Fe28 are as
Name and formulaReference code: PDF index name: Empirical
formula: Chemical formula: 00-003-1053 Boron Iron BFe2 Fe2B
Crystal system: Space group: Space group number: a (A): b (A): c
(A): Alpha (): Beta (): Gamma (): Volume of cell: Z: RIR:
Tetragonal 14/mcm 140 5.0990 5.0990 4.2400 90.0000 90.0000
90.0000 110.24 4.00
Status, subfiles and qualityStatus: Subfiles: Quality: Marked as
deleted by 1CDD Inorganic Alloy, metal or intermetalic Common Phase
CommentsDeleted by: Deleted by 36 1332. Source of Unit Cell
Data: powder diffraction.-
ReferencesPrimary reference: The Dow Chemical Company., Private
1. Davis, J. R. (2002). Bonding. Surface Hardening of Steels -
Understanding the Basics. Ohio:ASM International, 213-226. 2.
Sinha, A. K. (1991). Bonding (Boromzing). Heat Treatment Vol., ASM
Handbook. Ohio:ASM International, 437-447. 3. Stewart, K. (1997).
Boromzing Protects Metals Against Wear. Adv. Mater. Process.,
155(3), 23-25. 4. Kulka, M. & Pertek, A. (2003). Microstructure
and properties of bonded 41Cr4 steel after laser surface
modification with re-melting. Appal. Surf. Sci., 214, 278-288. 5.
Anthymidis, K.G., Stergioudis, E., & Tsipas, D.N. (2001).
Bonding in a fluidized bed reactor. Mater. Lett., 51, 156-160. 6.
Anthymidis, K.G., Zinoviadis, P., Roussos, D. & Tsipas, D.N.
(2002). Bonding of nickel in a fluidized bed reactor. Mater. Res.
Bull., 37, 515-522. 7. Anthymidis, K.G., Stergioudis, G., &
Tsipas, D.N. (2002). Boride coatings on nonferrous materials in a
fluidized bed reactor and their properties. Sci. Technol. of Adv.
Mater., 3, 303-311. 8. Bourithis, L., Papaefthymiou, S. &
Papadimitriou, G.D. (2002). Plasma transferred arc bonding of a low
carbon steel: microstructure and wear properties. Appal. Surf.
Ski., 200, 203-218. 9.
transferred arc process using boron and chromium boride powders:
microstructure and wear properties. Mater. Lett., 57,
10. Yu, L.G., Khor, K.A. & Stmdararajan, G. (2002). Bonding
of mild steel using the spark plasma sintering (SPS) technique.
Surf. Coat. Technol., 157, 226-230. 11. Cabeo, E.R., Laudien, G.,
Biemer, S., Rie, K. -T. & Hoppe, S. (1999). Plasmaassisted
bonding of industrial components in a pulsed d.c. glow discharge.
Surf. Coat. Technol. 116-119, 229-233. 12. LObig, G. & Hunger,
H. -J. (1997). Generation of boride layers on steel and nickel
alloys by plasma activation of boron trifluoride. Thin Solid Films,
13.8artsch, K. & Leonhardt, A. (1999). Formation of iron
boride layers on steel by d.c.plasma boarding and deposition
processes. Surf Coat. Technol., 116-119, 386390. 14. Yoon, J. H.,
Mee, Y. K. & Lee, S.Y. (1999). Plasma paste boromzing treatment
of the stainless steel AISI 304. Surf. Coat. Technol., 112, 71-75.
15. Davis, M.A. , Wilbur, P.M., Williamson, D.L., Wei, R. &
Vajo, M.M. (1998). Ion implantation boarding of iron and AISI M2
steel using a high-current density, low energy, broad-bewn ion
source. Surf. Coat. Technol., 103-104, 52-57. 16. Sen, U., Sen, S.
& Yilmaz, F. (2004). Structural characterization of boride
layer on boronized ductile irons. Surf Coat. Technol., 176,
222-228. 17. Genel, K., Uzbek, I., Kurt, A. & 8indal C. (2002).
Boarding response of AISI W1 steel and use of artificial neural
network for prediction of boride layer properties. Surf. Coat.
Technol., 160, 38-43. 18. Uzbek, I., Konduk, B.A., Bindal, C. &
Ucisik A.H. (2002). Characterization of boride AISI 316L stainless
steel implant. Vacuum, 65, 521-525. 19. Uzbek, I. & Bindal, C.
(2002). Mechanical properties of boromzed AISI W4 steel. Surf.
Coat. Technol., 154, 14-20. 20. Zakhariev, Z., Marinov, M.,
Ziateva, R. & Khristov, KH. (1987). A new combination of
coatings on carbide cutting tools. Surf Coat. Technol., 31,
265-271. 21. Uzbek, I., Akbulut, H., Zeytin, S., Bindal, C., &
Ucisik, A.H. (2000). The characterization of boride 99.5% purity
nickel. Surf. Coat. Technol., 126, 166170. 22. Bindal, C. &
Ucisik, A.H. (1999). Characterization of brides formed on
impuritycontrolled chromium-based low alloy steels. Surf. Coat.
Technol., 122, 208-213. 23. Lee, S.Y., Kim, G.S. & Kim, B.-S.
(2004). Mechanical properties of duplex layer formed on AISI 403
stainless steel by chromizing and boronizing treatment. Surf Coat.
Technol., 177-178, 178-184. 24. Maragoudakis, N.E., Stergioudis,
G., Omar, H., Pavlidou, E. & Tsipas, D.N. (2002).
Boro-nitriding of steel US 37-1. Mater. Lett., 57, 949-952. 25.
Gidikova, N. (1999). Vanadium boride coatings on steel. Mater. Sci.
Eng. A, 278, 181-186. 26. Yan, P.X. & Su, Y.C. (1995). Metal
surface modification by B-C-nitriding in a twotemperature-stage
process. Mater. Chem. Phys., 39, 304-308.
53 27. Kulka M. & Pertek A. (2003). Characterization of
complex (B + C + N) diffusion layers formed on chromium and
nickel-based low-carbon steel. Appl. Surf. Sc., 218, 114-123. 28.
Pertek, A. & Kulka, M. (2003). Two-step treatment carburizing
followed by boarding on medium-carbon steel. Surf Coat Technol.,
173, 309-314. 29. Zakhariev, Z. & Zlateva, R. (1993). Gas phase
reactions during simultaneous boronizing and aluminizing of steels.
J. Alloys Comp., 196, 59-62. 30. Ziateva, R.S. & Zakhariev,
Z.T. (1993). Structure of boromzing layers on steels. Bulge. Chem.
Comm., 26(1), 82-89. 31. Maragoudakis, N. E., Stergioudis, G.,
Omar, H., Paulidou, H. & Tsipas D.N. (2002). Boron-aluminide
coatings applied by pack cementation method on low-alloy steels.
Mater. Lett., 53, 406-410. 32. Wierzchon, T., Bielinski, P. &
Sikorski, K. (1995). Formation and properties of multicomponent and
composite boride layers on steel. Surf. Coat. Technol., 73,
121-124. 33. Darnley, P. A. & Bell, T. (1985). Engineering the
surface with boron based materials. Surface Engineering, 1(3),
34. Chatterjee-Fischer, R. (1989). Boarding and Diffusion
Metallizing. Surface Modification Technologies. New York:Marcel
Dekker, Inc., 567-609. 35. Palombarini, G. and Carbucicchio, M.
(1984). On the morphology of thermochemically produced Fe28/Fe
interfaces. J. Mater. Sci. Lett., 3 , 791-794. 36. Palombarini, G.
and Carbucicchio, M. (1987). Growth of bride coatings on iron. J.
Mater. Sci. Lett., 6, 415-416. 37. Htmger, H. J. & Trute, G.
(1994). Boromzing to Produce Wear-resistant Surface Layers. Heat
Treatment of Metals, 2, 31-39. 38. Budinski, K. (1988). Surface
Engineering for Wear Resistance, Prentice-Hall, 303345. 39.
Skugorova, L. P., Shylkov, V.1. & Netschaev, A. I. (1972).
Apparatus and technology of gas borating. Metalloved. Term. Obra.
Met., 5, 61-62. 40. Raveh A., Inspektor A., Carpi, U. & Avni R.
(1983). Boromzation of titanium and steels in a low pressure r.f.
plasma. Thin Solid Film, 108, 39-45.
54 41. Pasechnik, S.Y. et al. (1972). Protective Coatings on
Metals, Vol.4. New York: Consultants Bureau, 37-40. 42. Kaidash,
N.G. et al. (1972). Protective Coatings on Metals, Vol.4. New
York:Consultants Bureau, 149-155. 43. Chatterjee-Fischer, R.
(1981). Nitriding and nitrocarburizing Part V. Hart.-Tech. Mitt.,
36 (5), 248-254.